Textural properties of MMT, SPC, HPW-SPC-SG and HPW-SPC-IM samples. a The values were determined from N2 desorption isotherm. b The gallery height is defined as basal spacing minus the 0.96 nm thickness of MMT layer.
Because of the increasing environmental concern and legal requirements, it has been an urgent subject to find new processes for ultra-deep desulfurization of fuel oils. The conventional hydrodesulfurization (HDS) technique has some inherent problems in treating sulfur-containing aromatic hydrocarbon compounds, such as dibenzothiophene (DBT) and its derivatives. Thus, a large number of non-HDS processes, such as adsorption, extraction, oxidation, precipitation and bio-processes have been explored [1-7]. Among these methods, catalytic oxidative desulfurization (ODS) combined with extraction is regarded as the most promising and economical process [8-11]. The ODS process has been studied in various systems, including oxidant H2O2 with inorganic acids , organic acids [13-15], TS-1 , and heteropoly acids (HPA) catalysts [17-19]. HPA catalysts, especially those having the Keggin structure, have been determined to be very effective for the oxidation of sulfur-containing compounds in a liquid-liquid two-phase system. However, the separation and recovery of the catalysts are very difficult. For these reasons, the stable and water-tolerant solid acid catalysts have been developed. Li et al. , Lü et al. , and Gao et al.  reported [(C18H37)2N(CH3)2]3[PW12O40], [C18H37N(CH3)3]4[H2NaPW10O36], and Q[W(O)(O2)2(C5H4NCO2)] (Q=(C4H9)4N, [(CH3)3N(C18H37)] and [(C18H37)2N(CH3)2]) catalysts, respectively. Over these catalysts, DBT and its derivatives can be selectively oxidized into their corresponding sulfones using H2O2 as the oxidant in diesel oil. The surfactant-type catalysts provided a new process for deep ODS. However, the double long carbon chains of quaternary ammonium surfactant used in their system are very expensive.
In our previous works, monovacant lacunary Keggin-type polyoxometalate was introduced into mesoporous silica structure and showed high oxidation activity for ODS . Furthermore, we recently prepared a series of ordered mesoporous clay materials known as silica pillared clay (SPC) materials and metal ion doped SPC materials [24-29]. These inorganic porous materials with a controlled pore structure have stimulated a great deal of interest for their potential application as selective catalysts, adsorbents, separating agents, and porous matrixes for encapsulation of specific functional molecules [30-33].
In this study, in order to combine the porous advantages of the SPC and the appropriate acidity of H3PW12O40 (HPW) heteropoly acid, HPW was encapsulated into the ordered mesoporous SPC material by sol-gel method (denoted as HPW-SPC-SG) involving introduction of the HPW into clay interlayer template in an acidic suspension. The catalytic performance of the HPW-SPC-SG materials was studied through the ODS of the model oil. The results indicate that the HPW-SPC-SG materials exhibited high catalytic performance in ODS.
All solvents and reactants are commercially available and were used without further purification. The natural montmorillonite clay (MMT) was obtained from Inner Mongolia and used as the starting clay without any further purification or ions exchanging. The raw clay had a basal (001) spacing of 15.4 Å and an anhydrous structural (layer) formula of [Si7.86Al0.14][Al2.84Fe0.30Mg0.86]O20(OH)4, with a cation exchange capacity (CEC) of 91 meq/100 g .
2.0 g of MMT was first suspended in 120 mL of deionized water in a round bottom flask, to which 4.0 g of cetyltrimethylammonium bromide (CTAB) dissolved in 10.0 mL of pure ethanol was added dropwise and stirred for 1 h and a gel mixture was gained. Then, the pH of the gel was adjusted by HCl solution to 2.0. Subsequently, the calculated amount of H3PW12O40.6H2O was dissolved in 10.0 mL of water and added dropwise into the prepared gel under vigorous stirring. After the mixture was stirred for 4 h, 10.0 mL of tetraethyl orthosilicate (TEOS) was added, followed by stirring for 12 h at room temperature. And then, the mixture was put into an autoclave and heated for 24 h in a furnace at 110 °C. The autoclave was cooled, and the product was separated by filtration, throughly washed with deioined water, and dried in an oven at 110 °C. Then the dried samples were calcined at 500 oC for 6 h in a furnace. The samples were designated as
The SPC sample was prepared following the same procedure as the HPW-SPC-SG samples without the addition of HPW. And the impregnated samples were also prepared by an incipient wetness impregnation method using SPC as the support [34-36]. The loading amount of HPW was varied in the range of 5 to 25 wt.% by changing the concentration of the HPW in water. Typically, an aqueous HPW solution volume of 5 ml was used per gram of freshly calcined SPC. After impregnation, the wet samples were dried at 110 oC in an oven. The final HPW/SPC samples prepared by impregnation were denoted as
2.3. Catalytic performance in oxidative desulphurization
The model compound DBT was dissolved into
X-ray diffraction was performed on a Rigaku D/Max 2500 VBZ+/PC diffractometer using Cu-Kα radiation at low-angle range (2
3. Results and discussion
3.1. The formation mechanism of the HPW-SPC-SG samples
Scheme 1 illustrates the proposed formation mechanism of the HPW-SPC-SG materials. Firstly, MMT was suspended in aqueous solutions and ion-exchanged with surfactant CTAB. During this process, the surfactant formed micelle in the interlayer regions. Then, the pH of the mixture was adjusted by HCl solution to 2.0 and an appropriate amount of HPW was introduced into the solution. PW12O403- can substitute Br- and Cl- in the shell surrounding the micelle. Furthermore, the addition of HCl solution can keep the solution in a strong acidic environment to retain the Keggin-type HPW heteropoly acid intact. When TEOS was finally added into the gel mixture, it would intercalate into the clay interlayer regions by solvation and rapidly hydrolyze in acidic conditions to form the protonated H5SiO4+ monomers. The silicate cations would interact with the anionic shell surrounding the CTAB micelle to trap both X- (Cl-, Br-) and heteropoly anions, leading to the formation of a silica layer around the surfactant template. Thus, the heteropoly anions would be present at the interface between the silica and the CTAB micelle. During the long time stirring and hydrothermal treatment of the gel, the silica layer was polymerized and formed the Si-O-Si bonds between the interlayer regions. Washing and drying steps did not remove the heteropoly anions since they were trapped inside the clay interlayer. In the calcination step, the silica layer further condensed and yielded the completely cross-linked framework to strengthen the siloxanepillars and the mesopore structure, while the CTAB template decomposed and was eliminated from the pore system, but the HPW molecules remained fixed into the SPC frameworks .
3.2. The characterization of the samples
The small angle XRD patterns of the calcined MMT, SPC and HPW-SPC-SG samples are shown in Figure 1A. All the HPW-SPC-SG samples showed a broad characteristic (001) diffraction peak at about 2.0, which indicates that introducing HPW during the intercalation of CTAB did not destroy the SPC mesoporous lamellar structure. This result supports the proposed formation mechanism of the HPW-SPC-SG samples. The basal spacing and the gallery height of HPW-SPC-SG samples are summarized in Table 1. The HPW-SPC-SG materials exhibited refraction corresponding to a basal spacing of 4.38-4.47 nm. Since the thickness of the clay layer sheet is about 0.96 nm , the corresponding gallery heights are around 3.42-3.51 nm. Moreover, with theincrease of the HPW content, the refraction peak shifted to the low angle scope and the gallery height was found to increase gradually. This implies that the HPW has been encapsulated into the silica pillared frameworks of the SPC. However, with the introduction of more HPW, the XRD peaks became less resolved, as the 25%HPW-SPC-SG sample gave no obvious diffraction peak. This is because that the HPW is encapsulated into the SPC frameworks, while the excessive amount of HPW clog the pore passages .
The wide angle XRD patterns of the calcined MMT, SPC, HPW-SPC-SG, 15%HPW-SPC-IM and HPW samples are presented in Figure 1B. The SPC and the HPW-SPC-SG samples all showed the MMT characteristic peaks, which were assigned to (110), (020), (004), (130), (200), (330) and (060) diffractions [29, 40]. This ulteriorly approves that the laminated structure of MMT and the crystalline structure of the clay sheet have not been destroyed during the intercalation of HPW. However, with the increase of the HPW content, the HPW-SPC-SG samples gradually showed some characteristic peaks of HPW crystal, which was obvious for the 25%HPW-SPC-SG sample. The phenomenon indicates that the excess amount of HPW was introduced into the interlayer, but the HPW was not highly dispersed in the mesoporous SPC [41, 42]. On the other hand, the characteristic peaks of HPW in the pattern of 15%HPW-SPC-IM sample can be evidently seen. The results indicate that HPW is much more highly dispersed in the HPW-SPC-SG samples than that in the HPW-SPC-IM samples.
The TG-DTA curves of the SPC, HPW and HPW-SPC-SG samples before calcination in the region of 30-800 oC are shown in Figure 2. For all the samples, the weight loss below 100 °C was attributed to the loss of the physisorbed H2O. There was a weight loss peak in the range of 210-500 °C for the SPC sample (Figure 2a), which was due to the decomposition of CTAB in the sample. The corresponding DTA curve indicated that CTAB template elimination was associated with a sharp exothermic peak centered at 323 °C . Another endothermic peak in the DTA diagram centered at 706 °C was corresponding to the collapse of the mesoporous gallery structure .
For the pure HPW (Figure 2b), there was an endothermic peak in the temperature range of 100-320 °C(weight loss 3.57%) centered at 215 oC in the DTA diagram, accounting for the loss of 6 H2O molecules per Keggin unit of the HPW. The endothermic peak also appeared in the DTA diagrams of the HPW-SPC-SG samples (Figure 2c, d, e). The exothermic peak of HPW beginning at 538 °C in the DTA curve is assigned to the decomposition of heteropoly acid to form mixed oxides [45, 46]. The appreciable exothermic peak was also observed between 538-592 oC in the DTA diagrams of the HPW-SPC-SG samples (Figure 2c, d, e), indicating that the HPW-SPC-SG materials did not lower the thermal stability of the HPW heteropoly acid.
For the HPW-SPC-SG samples, besides the exothermic peaks at 323 °C, there was another exothermic peak centered at 407 °C in the DTA diagram (Figure 2c, d, e), which was also attributed to the decomposition of CTAB . The decomposition of the organic cation extending to a higher temperature was due to the interactions of the CTAB and the HPW. Furthermore, the endothermic peak corresponding to the collapse of the mesoporous gallery structure also appeared in the DTA diagram of the HPW-SPC-SG samples (Figure 2c, d, e). This implies that the incorporation of the HPW did not destroy the interlayer gallery structures of the HPW-SPC-SG samples. The TG-DTA curves also show that the HPW-SPC-SG samples can be obtained after treating the gels at 500 °C for 6h.
The FT-IR spectra of the pure HPW, SPC and HPW-SPC-SG samples in the region of 1400-600 cm-1 are shown in Figure 3. The spectrum of the HPW showed a broadened band at 802 cm−1, which was assigned to
The nitrogen adsorption/desorption isotherms and the mesoporous size distribution of the HPW-SPC-SG samples are shown in Figure 4. All samples presented type IV isotherm patterns with H3-type hysteresis loop starting at about 0.4 partial pressure, which are the characteristics of the mesoporous materials with the cylindrical pores formed in gallery regions . For the 25%HPW-SPC-SG sample, the hysteresis loop of the isotherm was obviously smaller than that of the samples with relatively low HPW contents. Furthermore, the desorption branch of the sample extended to a relatively lower pressure, suggesting a partial loss of structural organization and the formation of some narrower slit-shaped pores . Nevertheless, the main part of the hysterese was still between
The mesoporous pore size distribution is depicted in the inset of Figure 4. The results also indicate that all the HPW-SPC-SG samples have about the same pore diameters around 4.46-4.52 nm, which are slightly smaller than that of the SPC sample (5.06 nm). In the sol-gel synthesis method, the size of the majority of mesopores is formed by the CTAB micelle and the interclayer space, which is affected scarcely by the presence of HPW. This is in agreement with the proposed formation mechanism (Scheme 1). On the contrary, the pore diameters of the HPM-SPC-IM samples are reduced to about 4.33-3.82 nm, which indicates that HPW inside the mesopores occupied the space and decreases the pore width .
|Basal spacing (nm)||Gallery heightb (nm)|
The SEM images of the SPC, HPW-SPC-SG and 15%HPW-SPC-IM samples are shown in Figure 5. The SPC sample exhibited a slightly swelled nature mortmorillite plates morphology , while all the HPW-SPC-SG samples also exhibited plates structure, which was similar to the morphologies of the SPC sample. Though there were more fragmental particles with the increase of the HPW content in the HPW-SPC-SG samples, the main laminated structures of the HPW-SPC-SG samples were still retained, which indicates that the interlayer gallery structures were unaffected by the incorporation of the HPW. The 15 wt.% HPW-SPC-IM sample also retained a mortmorillite lamellar structure, though the HPW has an impact on the surface of the lamellar structure.
3.3. Catalytic performance of oxidizing modle oil
The effect of the reaction time on the ODS of the modle oil with sulfur content of 500 ppm over the HPW-SPC-SG catalysts is shown in Figure 6. It is obvious that the sulfur removal over 5%HPW-SPC-SG, 15%HPW-SPC-SG and 25%HPW-SPC-SG catalysts can reach up to 97.6%, 97.8% and 95.8% within 80 min, respectively. The results indicate that the HPW-SPC-SG samples are highly efficient in catalytic ODS of the DBT. But the 25%HPW-SPC-SG sample exhibited comparatively lower activity than the 15%HPW-SPC-SG sample, this is because the presence of high HPW contents leads to the decrease of the
The sulfur removal of the model oil over the 15%HPW-SPC-SG catalyst with reaction time at different temperatures is shown in Figure 7. The sulfur removal appeared to be unsatisfying at a temperature of 40 °C, which may be because H2O2 and the catalyst cannot work efficiently under low reaction temperature. Raising the reaction temperature from 40 to 60 °C led to a remarkable increase in the sulfur removal. However, further increase of the reaction temperature to 70 °C caused the decrease of the desulfurization efficiency. This is because the high temperature leads to the partial decomposition of H2O2, which brings down the oxidation effeciency. But the sulfur removal at 70 °C was still higher than that at 50 °C, which indicates that a proper increase of temperature favores the ODS of DBT.
Table 2 shows the results of the sulfur removal of the model oil over different catalysts. The results indicated that direct extraction without oxidation resulted in lower sulfur removal. And the catalytic activity of the HPW-SPC-SG samples was better than that of the HPW-SPC-IM samples. This is because the
|Catalysts||S remaining (E)a (ppm)||S remaining (ppm)||S removal (%)|
|SPC (0% HPW)||154.3||148.8||70.2|
The HPW-SPC-SG materials were successfully prepared by sol-gel method. The catalysts showed a homogeneous dispersion of the HPW molecules even at 25 wt.% loading. HPW was encapsulated into the gallery silica framework structure in the HPW-SPC-SG samples. The HPW-SPC-SG materials showed better catalytic performance for ODS of the oil than that of the HPW-SPC-IM samples. Under the optimized conditions, the sulfur content in the model oil can be reduced from 500 to 7.1 ppm. The prepared HPW-SPC-SG materials are promising and efficient catalysts for ODS of fuel oils.
The work was financially supported by the National Basic Research Program of China (973 Program, Grant No. 2011CBA00506).
Yang R. T. Hernández-Maldonado A. J. Yang F. H. 2003Science 30179.
Tao H. Nakazato T. Sato S. 2009Fuel 88 1961.
Shiraishi Y. Tachibana K. Hirai T. Komasawa I. 2002Ind. Eng. Chem. Res. 41 4362.
Murata S. Murata K. Kidena K. Nomura M. 2004Energy Fuels 18 116.
Babich I. V. Moulijn J. A. 2003Fuel 82 607.
Ito E. Rob J. A. van Veen 2006Catal. Today 116 446.
Song C. Ma X. 2003Appl. Catal. B: Environ. 41 207.
Sharipov A. K. Nigmatullin V. R. 2005Pet. Chem. 45 371.
Sharipov A. Nigmatullin V. Nigmatullin I. Zakirov R. 2006Fuels Oils 42 451.
Anisimov A. Tarakanova A. Russ 2009J. Gen. Chem. 79 1264.
Campos-Martin J. M. Capel-Sanchez M. C. Perez-Presas P. Fierro J. L. G. 2010J. Chem. Technol. Biotechnol. 85 879.
Tam P. S. Kittrell J. R. Eldridge J. W. 1990Ind. Eng. Chem. Res. 29 (1990) 321.
Yu G. X. Lu S. X. Chen H. Zhu Z. 2005Carbon 43 2285.
Al-Shahrani F. Xiao T. C. Llewellyn S. A. Barri S. Jiang Z. Shi H. H. Martinie G. Green M. L. H. 2007Appl. Catal. B: Environ. 73 311.
Filippis P. D. Scarsella M. 2003Energy Fuels 17 1452.
Kong L. Y. Li G. Wang X. S. Wu B. 2006Energy Fuels 20 896.
Te M. Fairbridge C. Ring Z. 2001Appl. Catal. A: Gen. 219 267.
Li H. M. He L. N. Lu J. D. Zhu W. S. Jiang X. Wang Y. Yan Y. S. 2009Energy Fuels 23 1354.
Arias M. Laurenti D. Geantet C. Vrinat M. Hideyuki I. Yoshimura Y. 2008Catal. Today 130 190.
Li C. Jiang Z. Gao J. Yang Y. Wang S. Tian F. Sun F. Sun X. Ying P. Han C. 2004Chem. Eur. J. 10 2277.
Lü H. Y. Gao J. Jiang Z. X. Jing F. Yang Y. X. Wang G. Li C. 2006J. Catal. 239 369.
Gao J. B. Wang S. G. Jiang Z. X. Lu H. Y. Yang Y. X. Jing F. Li C. 2006J. Mol. Catal. A: Chem. 258 261.
Abdalla Z. E. A. Li B. S. Tufail A. 2009Colloids Surf. A: Physicochem. Eng. Aspects 341 86.
Mao H. H. Li B. S. Li X. Liu Z. X. Ma W. 2009Appl. Surf. Sci. 255 4787.
Li B. S. Mao H. H. Li X. Ma Liu W. Z. X. 2009J. Collid. Interface. Sci. 336 244.
Mao H. H. Li B. S. Li X. Liu Z. X. Ma W. 2009Mater. Res. Bull. 44 1569.
Mao H. H. Li B. S. Li X. Liu Z. X. Ma W. 2009Catal. Commun. 10 975.
Mao H. H. Li B. S. Li X. Yue L. W. Liu Z. X. Ma W. 2010Ind. Eng. Chem. Res. 49 583.
Mao H. H. Li B. S. Li X. Yue L. W. 2010Micropor. Mesopor. Mater. 130 314.
Ishida H. Campbell S. Blackwell J. 2000Chem. Mater. 12 1260.
Horch R. A. Golden T. D. D’Souza N. A. Riester L. 2002Chem. Mater. 14 3531.
Zhu H. Y. Zhao J. C. Liu J. W. Yang X. Z. Shen Y. N. 2006Chem. Mater. 18 3993.
Juan J. C. Zhang J. C. Yarmo M. A. 2007J. Mol. Catal. A: Chem. 267 265.
Miyaji A. Echizen T. Nagata K. Yoshinaga Y. Okuhara T. 2003J. Mol. Catal. A: Chem. 201 145.
Sugii T. Ohnishi R. Zhang J. Miyaji A. Kamiya Y. Okuhara T. 2006Catal. Today 116 179.
Xia Q. H. Hidajat K. Kawi S. 2002J. Catal. 209 433.
Gagea B. C. Lorgouiloux Y. Altintas Y. Jacobs P. A. Martens J. A. 2009J. Catal. 265 99.
Pluta M. Galeski A. Alexandre M. M. Paul A. Dubois P. 2002J. Appl. Polym. Sci. 86 1497.
Toufaily J. Soulard M. Guth J. L. Patarin J. Delmote L. Hamieh T. Kodeih M. Naoufal D. Hamad H. 2005Colloids Surf. A: Physicochem. Eng. Aspects 316 285.
Bracco S. Valsesia P. Ferretti L. Sozzani P. Mauri M. Comotti A. 2008Micropor. Mesopor. Mater. 107 102.
Ghanbari-Siahkali A. Philippou A. Dwyer J. Anderson M. W. 2000Appl. Catal. A: Gen. 192 57.
Kukovecz Á. Zs Balogi. Z. Kónya M. Tobab P. Lentzc S. I. Niwa F. Mizukami Á. Molnárd J. B. Nagyc I. Kiricsi 2002Appl. Catal. A: Gen. 228 83.
Kleitz F. Schmidt W. Schüth F. 2003Micropor. Mesopor. Mater. 65 1.
Occelli M. L. 1983Ind. Eng. Chem. Prod. Res. Dev. 22 553.
Kozhevnikov I. V. 2007J. Mol. Catal. A: Chem. 262 86.
Ajaikumar S. Pandurangan A. 2008J. Mol. Catal. A: Chem. 286 21.
Gamelas J. A. Couto F. A. S. Trova M. C. N. Äo A. M. V. Cavaleiro J. A. S. Cavaleiro J. D. Pedrosa de Jesus. 1999Thermochim. Acta 326 165.
Rocchiccioli-Deltcheff C. Foumier M. Frank R. 1983Inorg. Chem. 22 207.
Zhu H. Y. Ding Z. Barry J. C. 2002J. Phys. Chem. B 106 11420.
Hu L. H. Ji S. F. Jiang Z. Song H. L. Wu P. Y. Liu Q. Q. 2007J. Phys. Chem. C 111 15173.
Bordoloi A. Lefebvre F. Halligudi S. B. 2007J. Catal. 247 166.
Rojas F. Kornhauser I. Felipe C. Esparza J. M. Cordero S. Dominguez A. Riccardo J. L. 2002Phys. Chem. Chem. Phys. 4 2346.